#------------------------------------------------------------------------------
#$Date: 2023-06-29 13:54:23 +0300 (Thu, 29 Jun 2023) $
#$Revision: 284616 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/32/7713276.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7713276
loop_
_publ_author_name
'Shang, Jining'
'Li, Xiang'
'Ren, Yuanhang'
'Ding, Hongxin'
'Cao, Jiapeng'
'He, Rui'
'Yue, Bin'
'He, Heyong'
_publ_section_title
;
 An one-dimensional chain of manganese(II) bridged peroxomolybdate
 isolated from aqueous Mn-polymolybdate-H2O2 system
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D3DT01243C
_journal_year                    2023
_chemical_formula_sum            'Cs8 Mn2 Mo14 O65'
_chemical_formula_weight         3556.32
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   23.5716(17)
_cell_length_b                   10.7966(8)
_cell_length_c                   12.5938(9)
_cell_measurement_reflns_used    9895
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      55.10
_cell_measurement_theta_min      4.47
_cell_volume                     3205.0(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_radiation_type           GaK\a
_diffrn_radiation_wavelength     1.34138
_diffrn_reflns_av_R_equivalents  0.0878
_diffrn_reflns_av_unetI/netI     0.0364
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            38979
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        53.594
_diffrn_reflns_theta_max         55.163
_diffrn_reflns_theta_min         3.262
_exptl_absorpt_coefficient_mu    41.593
_exptl_absorpt_correction_T_max  0.012
_exptl_absorpt_correction_T_min  0.002
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.685
_exptl_crystal_density_meas      3.704
_exptl_crystal_description       block
_exptl_crystal_F_000             3770
_exptl_crystal_size_max          0.150
_exptl_crystal_size_mid          0.080
_exptl_crystal_size_min          0.060
_refine_diff_density_max         5.727
_refine_diff_density_min         -4.579
_refine_diff_density_rms         0.443
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         3235
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.089
_refine_ls_R_factor_all          0.0652
_refine_ls_R_factor_gt           0.0614
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0849P)²+175.1546P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1674
_refine_ls_wR_factor_ref         0.1764
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3088
_reflns_number_total             3235
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3dt01243c3.cif
_cod_data_source_block           ga_200721ca_a
_cod_database_code               7713276
_shelx_shelxl_version_number     2016/6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.032
_shelx_estimated_absorpt_t_max   0.095
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.63230(6) 0.250000 0.22629(10) 0.0097(3) Uani 1 2 d S T P . .
Mo2 Mo 0.62860(4) 0.44422(9) 0.44242(8) 0.0133(3) Uani 1 1 d . . . . .
Mo3 Mo 0.52203(4) 0.44807(9) 0.27772(8) 0.0143(3) Uani 1 1 d . . . . .
Mo4 Mo 0.73052(6) 0.250000 0.41630(11) 0.0146(3) Uani 1 2 d S T P . .
Mo5 Mo 0.50971(6) 0.250000 0.09307(11) 0.0140(3) Uani 1 2 d S T P . .
Mn1 Mn 0.58569(13) 0.750000 0.3446(2) 0.0160(6) Uani 1 2 d S T P . .
Cs1 Cs 0.57627(7) 0.250000 0.72927(12) 0.0414(4) Uani 1 2 d S T P . .
Cs2 Cs 0.61580(5) -0.03525(13) 0.01071(13) 0.0593(5) Uani 1 1 d . . . . .
Cs3 Cs 0.64481(6) 0.750000 0.64537(10) 0.0315(4) Uani 1 2 d S T P . .
O1 O 0.6437(5) 0.250000 0.4080(9) 0.012(2) Uani 1 2 d S T P . .
O2 O 0.5349(5) 0.250000 0.2498(9) 0.011(2) Uani 1 2 d S T P . .
O3 O 0.7078(4) 0.4267(9) 0.4029(7) 0.0169(19) Uani 1 1 d . . . . .
O4 O 0.6162(4) 0.0876(9) 0.2649(7) 0.0149(18) Uani 1 1 d . . . . .
O5 O 0.5499(4) 0.4114(8) 0.4214(7) 0.0164(18) Uani 1 1 d . . . . .
O6 O 0.6129(6) 0.250000 0.0934(10) 0.018(3) Uani 1 2 d S T P . .
O7 O 0.5217(4) 0.4253(8) 0.1296(7) 0.0176(19) Uani 1 1 d . . . . .
O8 O 0.7054(5) 0.250000 0.2308(10) 0.017(3) Uani 1 2 d S T P . .
O9 O 0.6287(4) 0.6061(9) 0.4259(8) 0.022(2) Uani 1 1 d . . . . .
O10 O 0.6341(4) 0.4228(10) 0.5745(7) 0.023(2) Uani 1 1 d . . . . .
O11 O 0.6498(7) 0.750000 0.2176(12) 0.034(4) Uani 1 2 d S T P . .
O12 O 0.5356(4) 0.6067(9) 0.2763(7) 0.022(2) Uani 1 1 d . . . . .
O13 O 0.7415(7) 0.250000 0.5478(11) 0.025(3) Uani 1 2 d S T P . .
O14 O 0.8019(4) 0.3187(10) 0.3630(9) 0.030(2) Uani 1 1 d . . . . .
O15 O 0.4520(4) 0.4335(10) 0.3042(9) 0.030(2) Uani 1 1 d . . . . .
O16 O 0.4387(6) 0.250000 0.1078(11) 0.023(3) Uani 1 2 d S T P . .
O17 O 0.5188(5) 0.1835(11) -0.0476(8) 0.036(3) Uani 1 1 d . . . . .
O18 O 0.5227(6) 0.750000 0.4737(11) 0.023(3) Uani 1 2 d S T P . .
O19 O 0.7597(6) 0.6057(19) 0.5277(13) 0.070(5) Uani 1 1 d . . . . .
O20 O 0.7325(5) -0.0512(11) 0.2090(9) 0.035(3) Uiso 1 1 d . . . . .
O22 O 0.688(2) 0.302(5) 0.828(4) 0.046(12) Uiso 0.25 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.1739 6.3004 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn -0.0162 2.2332 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -0.2130 2.1496 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0389 0.0241 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 Mo1 O6 107.2(6) . . ?
O8 Mo1 O4 101.2(3) . . ?
O6 Mo1 O4 101.5(3) . . ?
O8 Mo1 O4 101.2(3) . 7_565 ?
O6 Mo1 O4 101.5(3) . 7_565 ?
O4 Mo1 O4 141.3(5) . 7_565 ?
O8 Mo1 O1 81.4(5) . . ?
O6 Mo1 O1 171.4(5) . . ?
O4 Mo1 O1 76.3(3) . . ?
O4 Mo1 O1 76.3(3) 7_565 . ?
O8 Mo1 O2 170.8(5) . . ?
O6 Mo1 O2 82.1(5) . . ?
O4 Mo1 O2 76.4(3) . . ?
O4 Mo1 O2 76.4(3) 7_565 . ?
O1 Mo1 O2 89.4(4) . . ?
O8 Mo1 Cs2 96.7(3) . 7_565 ?
O6 Mo1 Cs2 48.70(6) . 7_565 ?
O4 Mo1 Cs2 149.0(3) . 7_565 ?
O4 Mo1 Cs2 56.5(3) 7_565 7_565 ?
O1 Mo1 Cs2 131.67(3) . 7_565 ?
O2 Mo1 Cs2 89.5(2) . 7_565 ?
O8 Mo1 Cs2 96.7(3) . . ?
O6 Mo1 Cs2 48.70(6) . . ?
O4 Mo1 Cs2 56.5(3) . . ?
O4 Mo1 Cs2 149.0(3) 7_565 . ?
O1 Mo1 Cs2 131.67(3) . . ?
O2 Mo1 Cs2 89.5(2) . . ?
Cs2 Mo1 Cs2 96.62(6) 7_565 . ?
O10 Mo2 O9 104.6(5) . . ?
O10 Mo2 O5 100.8(4) . . ?
O9 Mo2 O5 99.7(4) . . ?
O10 Mo2 O3 99.5(4) . . ?
O9 Mo2 O3 93.7(4) . . ?
O5 Mo2 O3 151.9(4) . . ?
O10 Mo2 O1 93.0(5) . . ?
O9 Mo2 O1 159.3(4) . . ?
O5 Mo2 O1 87.3(4) . . ?
O3 Mo2 O1 72.4(4) . . ?
O10 Mo2 O4 163.2(4) . 7_565 ?
O9 Mo2 O4 91.9(4) . 7_565 ?
O5 Mo2 O4 73.2(3) . 7_565 ?
O3 Mo2 O4 81.8(3) . 7_565 ?
O1 Mo2 O4 71.3(4) . 7_565 ?
O10 Mo2 Mo4 87.3(4) . . ?
O9 Mo2 Mo4 129.5(3) . . ?
O5 Mo2 Mo4 126.4(3) . . ?
O3 Mo2 Mo4 35.8(3) . . ?
O1 Mo2 Mo4 39.2(3) . . ?
O4 Mo2 Mo4 84.1(2) 7_565 . ?
O10 Mo2 Cs3 59.9(4) . . ?
O9 Mo2 Cs3 44.8(3) . . ?
O5 Mo2 Cs3 108.6(3) . . ?
O3 Mo2 Cs3 98.3(3) . . ?
O1 Mo2 Cs3 150.2(3) . . ?
O4 Mo2 Cs3 136.7(2) 7_565 . ?
Mo4 Mo2 Cs3 120.62(4) . . ?
O10 Mo2 Cs1 30.3(4) . . ?
O9 Mo2 Cs1 125.2(3) . . ?
O5 Mo2 Cs1 75.5(3) . . ?
O3 Mo2 Cs1 116.0(3) . . ?
O1 Mo2 Cs1 75.3(3) . . ?
O4 Mo2 Cs1 134.8(2) 7_565 . ?
Mo4 Mo2 Cs1 88.99(4) . . ?
Cs3 Mo2 Cs1 84.22(3) . . ?
O15 Mo3 O12 105.9(5) . . ?
O15 Mo3 O7 100.3(5) . . ?
O12 Mo3 O7 96.8(4) . . ?
O15 Mo3 O5 97.2(5) . . ?
O12 Mo3 O5 98.4(4) . . ?
O7 Mo3 O5 152.6(4) . . ?
O15 Mo3 O2 94.4(5) . . ?
O12 Mo3 O2 158.9(5) . . ?
O7 Mo3 O2 73.3(4) . . ?
O5 Mo3 O2 84.5(4) . . ?
O15 Mo3 O4 163.2(4) . 7_565 ?
O12 Mo3 O4 89.2(4) . 7_565 ?
O7 Mo3 O4 84.9(3) . 7_565 ?
O5 Mo3 O4 72.7(3) . 7_565 ?
O2 Mo3 O4 71.7(4) . 7_565 ?
O15 Mo3 Mo5 89.6(4) . . ?
O12 Mo3 Mo5 132.2(3) . . ?
O7 Mo3 Mo5 35.4(3) . . ?
O5 Mo3 Mo5 124.7(3) . . ?
O2 Mo3 Mo5 40.2(3) . . ?
O4 Mo3 Mo5 85.6(2) 7_565 . ?
O15 Mo3 Cs1 61.0(4) . 5_666 ?
O12 Mo3 Cs1 46.0(3) . 5_666 ?
O7 Mo3 Cs1 94.7(3) . 5_666 ?
O5 Mo3 Cs1 112.2(3) . 5_666 ?
O2 Mo3 Cs1 150.8(3) . 5_666 ?
O4 Mo3 Cs1 135.0(2) 7_565 5_666 ?
Mo5 Mo3 Cs1 118.69(4) . 5_666 ?
O15 Mo3 Cs2 134.7(4) . 7_565 ?
O12 Mo3 Cs2 70.7(3) . 7_565 ?
O7 Mo3 Cs2 39.2(3) . 7_565 ?
O5 Mo3 Cs2 128.1(3) . 7_565 ?
O2 Mo3 Cs2 91.0(3) . 7_565 ?
O4 Mo3 Cs2 57.0(2) 7_565 7_565 ?
Mo5 Mo3 Cs2 66.80(4) . 7_565 ?
Cs1 Mo3 Cs2 96.10(3) 5_666 7_565 ?
O13 Mo4 O14 101.9(6) . 7_565 ?
O13 Mo4 O14 101.9(6) . . ?
O14 Mo4 O14 44.6(6) 7_565 . ?
O13 Mo4 O3 97.2(3) . . ?
O14 Mo4 O3 124.5(4) 7_565 . ?
O14 Mo4 O3 80.7(4) . . ?
O13 Mo4 O3 97.2(3) . 7_565 ?
O14 Mo4 O3 80.7(4) 7_565 7_565 ?
O14 Mo4 O3 124.5(4) . 7_565 ?
O3 Mo4 O3 147.2(5) . 7_565 ?
O13 Mo4 O1 101.8(6) . . ?
O14 Mo4 O1 147.2(4) 7_565 . ?
O14 Mo4 O1 147.2(4) . . ?
O3 Mo4 O1 74.2(3) . . ?
O3 Mo4 O1 74.1(3) 7_565 . ?
O13 Mo4 O8 174.6(6) . . ?
O14 Mo4 O8 83.1(4) 7_565 . ?
O14 Mo4 O8 83.1(4) . . ?
O3 Mo4 O8 81.5(3) . . ?
O3 Mo4 O8 81.5(3) 7_565 . ?
O1 Mo4 O8 72.8(4) . . ?
O13 Mo4 Mo2 90.8(4) . . ?
O14 Mo4 Mo2 158.0(3) 7_565 . ?
O14 Mo4 Mo2 115.5(3) . . ?
O3 Mo4 Mo2 34.9(3) . . ?
O3 Mo4 Mo2 115.8(3) 7_565 . ?
O1 Mo4 Mo2 41.99(7) . . ?
O8 Mo4 Mo2 85.1(2) . . ?
O13 Mo4 Mo2 90.8(4) . 7_565 ?
O14 Mo4 Mo2 115.5(3) 7_565 7_565 ?
O14 Mo4 Mo2 158.0(3) . 7_565 ?
O3 Mo4 Mo2 115.8(3) . 7_565 ?
O3 Mo4 Mo2 34.9(3) 7_565 7_565 ?
O1 Mo4 Mo2 41.99(7) . 7_565 ?
O8 Mo4 Mo2 85.1(2) . 7_565 ?
Mo2 Mo4 Mo2 81.70(5) . 7_565 ?
O13 Mo4 Cs2 67.1(4) . 8_766 ?
O14 Mo4 Cs2 65.8(3) 7_565 8_766 ?
O14 Mo4 Cs2 36.6(3) . 8_766 ?
O3 Mo4 Cs2 75.1(2) . 8_766 ?
O3 Mo4 Cs2 137.7(3) 7_565 8_766 ?
O1 Mo4 Cs2 145.51(13) . 8_766 ?
O8 Mo4 Cs2 117.3(2) . 8_766 ?
Mo2 Mo4 Cs2 103.95(3) . 8_766 ?
Mo2 Mo4 Cs2 157.06(5) 7_565 8_766 ?
O13 Mo4 Cs2 67.1(4) . 2_655 ?
O14 Mo4 Cs2 36.6(3) 7_565 2_655 ?
O14 Mo4 Cs2 65.8(3) . 2_655 ?
O3 Mo4 Cs2 137.7(3) . 2_655 ?
O3 Mo4 Cs2 75.1(2) 7_565 2_655 ?
O1 Mo4 Cs2 145.51(13) . 2_655 ?
O8 Mo4 Cs2 117.3(2) . 2_655 ?
Mo2 Mo4 Cs2 157.06(5) . 2_655 ?
Mo2 Mo4 Cs2 103.95(3) 7_565 2_655 ?
Cs2 Mo4 Cs2 62.61(4) 8_766 2_655 ?
O13 Mo4 Cs3 130.4(5) . 2_664 ?
O14 Mo4 Cs3 34.8(3) 7_565 2_664 ?
O14 Mo4 Cs3 34.8(3) . 2_664 ?
O3 Mo4 Cs3 96.4(3) . 2_664 ?
O3 Mo4 Cs3 96.4(3) 7_565 2_664 ?
O1 Mo4 Cs3 127.8(3) . 2_664 ?
O8 Mo4 Cs3 55.0(3) . 2_664 ?
Mo2 Mo4 Cs3 124.53(4) . 2_664 ?
Mo2 Mo4 Cs3 124.53(4) 7_565 2_664 ?
Cs2 Mo4 Cs3 70.86(3) 8_766 2_664 ?
Cs2 Mo4 Cs3 70.86(3) 2_655 2_664 ?
O16 Mo5 O17 102.2(6) . 7_565 ?
O16 Mo5 O17 102.2(6) . . ?
O17 Mo5 O17 43.8(7) 7_565 . ?
O16 Mo5 O7 96.7(3) . . ?
O17 Mo5 O7 80.8(4) 7_565 . ?
O17 Mo5 O7 123.9(5) . . ?
O16 Mo5 O7 96.7(3) . 7_565 ?
O17 Mo5 O7 123.9(5) 7_565 7_565 ?
O17 Mo5 O7 80.8(4) . 7_565 ?
O7 Mo5 O7 148.1(5) . 7_565 ?
O16 Mo5 O2 100.5(6) . . ?
O17 Mo5 O2 148.2(4) 7_565 . ?
O17 Mo5 O2 148.2(4) . . ?
O7 Mo5 O2 74.6(3) . . ?
O7 Mo5 O2 74.6(3) 7_565 . ?
O16 Mo5 O6 173.6(6) . . ?
O17 Mo5 O6 83.7(5) 7_565 . ?
O17 Mo5 O6 83.7(5) . . ?
O7 Mo5 O6 81.7(3) . . ?
O7 Mo5 O6 81.7(3) 7_565 . ?
O2 Mo5 O6 73.1(4) . . ?
O16 Mo5 Mo3 90.6(4) . . ?
O17 Mo5 Mo3 114.4(4) 7_565 . ?
O17 Mo5 Mo3 156.4(4) . . ?
O7 Mo5 Mo3 33.6(3) . . ?
O7 Mo5 Mo3 117.6(3) 7_565 . ?
O2 Mo5 Mo3 43.26(6) . . ?
O6 Mo5 Mo3 84.7(2) . . ?
O16 Mo5 Mo3 90.6(4) . 7_565 ?
O17 Mo5 Mo3 156.4(4) 7_565 7_565 ?
O17 Mo5 Mo3 114.4(4) . 7_565 ?
O7 Mo5 Mo3 117.6(3) . 7_565 ?
O7 Mo5 Mo3 33.6(3) 7_565 7_565 ?
O2 Mo5 Mo3 43.26(6) . 7_565 ?
O6 Mo5 Mo3 84.7(2) . 7_565 ?
Mo3 Mo5 Mo3 84.76(5) . 7_565 ?
O16 Mo5 Cs2 45.3(3) . 5_655 ?
O17 Mo5 Cs2 89.9(3) 7_565 5_655 ?
O17 Mo5 Cs2 64.1(4) . 5_655 ?
O7 Mo5 Cs2 138.1(3) . 5_655 ?
O7 Mo5 Cs2 67.9(3) 7_565 5_655 ?
O2 Mo5 Cs2 121.9(2) . 5_655 ?
O6 Mo5 Cs2 138.08(15) . 5_655 ?
Mo3 Mo5 Cs2 134.55(5) . 5_655 ?
Mo3 Mo5 Cs2 85.18(4) 7_565 5_655 ?
O16 Mo5 Cs2 45.3(3) . 3_655 ?
O17 Mo5 Cs2 64.1(4) 7_565 3_655 ?
O17 Mo5 Cs2 89.9(3) . 3_655 ?
O7 Mo5 Cs2 67.9(3) . 3_655 ?
O7 Mo5 Cs2 138.1(3) 7_565 3_655 ?
O2 Mo5 Cs2 121.9(2) . 3_655 ?
O6 Mo5 Cs2 138.08(15) . 3_655 ?
Mo3 Mo5 Cs2 85.18(4) . 3_655 ?
Mo3 Mo5 Cs2 134.55(5) 7_565 3_655 ?
Cs2 Mo5 Cs2 71.27(5) 5_655 3_655 ?
O16 Mo5 Cs2 129.34(12) . 7_565 ?
O17 Mo5 Cs2 54.5(3) 7_565 7_565 ?
O17 Mo5 Cs2 88.8(4) . 7_565 ?
O7 Mo5 Cs2 41.4(3) . 7_565 ?
O7 Mo5 Cs2 133.9(3) 7_565 7_565 ?
O2 Mo5 Cs2 93.8(2) . 7_565 ?
O6 Mo5 Cs2 52.46(10) . 7_565 ?
Mo3 Mo5 Cs2 67.87(3) . 7_565 ?
Mo3 Mo5 Cs2 129.48(5) 7_565 7_565 ?
Cs2 Mo5 Cs2 143.89(4) 5_655 7_565 ?
Cs2 Mo5 Cs2 86.14(3) 3_655 7_565 ?
O9 Mn1 O9 94.3(5) . 7_575 ?
O9 Mn1 O12 173.7(4) . 7_575 ?
O9 Mn1 O12 85.8(4) 7_575 7_575 ?
O9 Mn1 O12 85.8(4) . . ?
O9 Mn1 O12 173.7(4) 7_575 . ?
O12 Mn1 O12 93.3(5) 7_575 . ?
O9 Mn1 O11 91.3(4) . . ?
O9 Mn1 O11 91.3(4) 7_575 . ?
O12 Mn1 O11 95.0(4) 7_575 . ?
O12 Mn1 O11 95.0(4) . . ?
O9 Mn1 O18 88.0(4) . . ?
O9 Mn1 O18 88.0(4) 7_575 . ?
O12 Mn1 O18 85.7(4) 7_575 . ?
O12 Mn1 O18 85.7(4) . . ?
O11 Mn1 O18 179.0(6) . . ?
O9 Mn1 Cs1 125.4(3) . 5_666 ?
O9 Mn1 Cs1 125.4(3) 7_575 5_666 ?
O12 Mn1 Cs1 50.6(3) 7_575 5_666 ?
O12 Mn1 Cs1 50.6(3) . 5_666 ?
O11 Mn1 Cs1 119.7(5) . 5_666 ?
O18 Mn1 Cs1 61.3(4) . 5_666 ?
O9 Mn1 Cs3 51.8(3) . . ?
O9 Mn1 Cs3 51.8(3) 7_575 . ?
O12 Mn1 Cs3 124.8(3) 7_575 . ?
O12 Mn1 Cs3 124.8(3) . . ?
O11 Mn1 Cs3 116.4(5) . . ?
O18 Mn1 Cs3 62.6(4) . . ?
Cs1 Mn1 Cs3 123.90(8) 5_666 . ?
O22 Cs1 O22 22(2) 7_565 . ?
O22 Cs1 O10 75.8(10) 7_565 7_565 ?
O22 Cs1 O10 89.2(10) . 7_565 ?
O22 Cs1 O10 89.2(10) 7_565 . ?
O22 Cs1 O10 75.8(10) . . ?
O10 Cs1 O10 76.2(4) 7_565 . ?
O22 Cs1 O12 132.8(10) 7_565 3_646 ?
O22 Cs1 O12 150.5(10) . 3_646 ?
O10 Cs1 O12 93.6(3) 7_565 3_646 ?
O10 Cs1 O12 133.3(3) . 3_646 ?
O22 Cs1 O12 150.5(10) 7_565 5_666 ?
O22 Cs1 O12 132.8(10) . 5_666 ?
O10 Cs1 O12 133.3(3) 7_565 5_666 ?
O10 Cs1 O12 93.6(3) . 5_666 ?
O12 Cs1 O12 60.8(4) 3_646 5_666 ?
O22 Cs1 O17 92.8(10) 7_565 7_566 ?
O22 Cs1 O17 88.0(10) . 7_566 ?
O10 Cs1 O17 153.5(3) 7_565 7_566 ?
O10 Cs1 O17 128.2(3) . 7_566 ?
O12 Cs1 O17 76.6(3) 3_646 7_566 ?
O12 Cs1 O17 62.7(3) 5_666 7_566 ?
O22 Cs1 O17 88.0(10) 7_565 1_556 ?
O22 Cs1 O17 92.8(10) . 1_556 ?
O10 Cs1 O17 128.2(3) 7_565 1_556 ?
O10 Cs1 O17 153.5(3) . 1_556 ?
O12 Cs1 O17 62.7(3) 3_646 1_556 ?
O12 Cs1 O17 76.6(3) 5_666 1_556 ?
O17 Cs1 O17 25.9(4) 7_566 1_556 ?
O22 Cs1 O18 155.4(10) 7_565 5_666 ?
O22 Cs1 O18 155.4(10) . 5_666 ?
O10 Cs1 O18 80.1(3) 7_565 5_666 ?
O10 Cs1 O18 80.1(3) . 5_666 ?
O12 Cs1 O18 53.3(2) 3_646 5_666 ?
O12 Cs1 O18 53.3(2) 5_666 5_666 ?
O17 Cs1 O18 111.3(3) 7_566 5_666 ?
O17 Cs1 O18 111.3(3) 1_556 5_666 ?
O22 Cs1 O15 92.1(10) 7_565 3_646 ?
O22 Cs1 O15 113.7(10) . 3_646 ?
O10 Cs1 O15 53.6(3) 7_565 3_646 ?
O10 Cs1 O15 127.6(3) . 3_646 ?
O12 Cs1 O15 48.7(2) 3_646 3_646 ?
O12 Cs1 O15 109.0(3) 5_666 3_646 ?
O17 Cs1 O15 104.1(3) 7_566 3_646 ?
O17 Cs1 O15 78.9(3) 1_556 3_646 ?
O18 Cs1 O15 77.47(18) 5_666 3_646 ?
O22 Cs1 O15 113.7(10) 7_565 5_666 ?
O22 Cs1 O15 92.1(10) . 5_666 ?
O10 Cs1 O15 127.6(3) 7_565 5_666 ?
O10 Cs1 O15 53.6(3) . 5_666 ?
O12 Cs1 O15 109.0(3) 3_646 5_666 ?
O12 Cs1 O15 48.7(3) 5_666 5_666 ?
O17 Cs1 O15 78.9(3) 7_566 5_666 ?
O17 Cs1 O15 104.1(3) 1_556 5_666 ?
O18 Cs1 O15 77.47(18) 5_666 5_666 ?
O15 Cs1 O15 154.0(4) 3_646 5_666 ?
O22 Cs1 Mn1 164.1(10) 7_565 5_666 ?
O22 Cs1 Mn1 164.1(10) . 5_666 ?
O10 Cs1 Mn1 106.6(2) 7_565 5_666 ?
O10 Cs1 Mn1 106.6(2) . 5_666 ?
O12 Cs1 Mn1 32.52(18) 3_646 5_666 ?
O12 Cs1 Mn1 32.52(18) 5_666 5_666 ?
O17 Cs1 Mn1 78.3(2) 7_566 5_666 ?
O17 Cs1 Mn1 78.3(2) 1_556 5_666 ?
O18 Cs1 Mn1 33.9(2) 5_666 5_666 ?
O15 Cs1 Mn1 77.69(17) 3_646 5_666 ?
O15 Cs1 Mn1 77.69(17) 5_666 5_666 ?
O7 Cs2 O16 103.9(3) 7_565 5_655 ?
O7 Cs2 O14 169.2(3) 7_565 8_755 ?
O16 Cs2 O14 65.4(3) 5_655 8_755 ?
O7 Cs2 O6 55.7(3) 7_565 . ?
O16 Cs2 O6 150.5(3) 5_655 . ?
O14 Cs2 O6 133.1(3) 8_755 . ?
O7 Cs2 O19 116.9(3) 7_565 8_755 ?
O16 Cs2 O19 139.1(4) 5_655 8_755 ?
O14 Cs2 O19 73.7(3) 8_755 8_755 ?
O6 Cs2 O19 64.1(4) . 8_755 ?
O7 Cs2 O17 46.6(3) 7_565 . ?
O16 Cs2 O17 98.1(3) 5_655 . ?
O14 Cs2 O17 130.3(3) 8_755 . ?
O6 Cs2 O17 52.5(3) . . ?
O19 Cs2 O17 107.1(4) 8_755 . ?
O7 Cs2 O4 51.3(2) 7_565 . ?
O16 Cs2 O4 138.3(3) 5_655 . ?
O14 Cs2 O4 138.0(2) 8_755 . ?
O6 Cs2 O4 48.8(3) . . ?
O19 Cs2 O4 76.2(3) 8_755 . ?
O17 Cs2 O4 86.3(2) . . ?
O7 Cs2 O11 93.4(3) 7_565 1_545 ?
O16 Cs2 O11 87.6(3) 5_655 1_545 ?
O14 Cs2 O11 88.2(3) 8_755 1_545 ?
O6 Cs2 O11 112.6(3) . 1_545 ?
O19 Cs2 O11 93.0(4) 8_755 1_545 ?
O17 Cs2 O11 139.9(3) . 1_545 ?
O4 Cs2 O11 64.8(2) . 1_545 ?
O7 Cs2 O17 56.2(3) 7_565 5_655 ?
O16 Cs2 O17 49.4(3) 5_655 5_655 ?
O14 Cs2 O17 113.7(3) 8_755 5_655 ?
O6 Cs2 O17 111.3(3) . 5_655 ?
O19 Cs2 O17 168.8(3) 8_755 5_655 ?
O17 Cs2 O17 75.0(3) . 5_655 ?
O4 Cs2 O17 93.1(2) . 5_655 ?
O11 Cs2 O17 79.3(3) 1_545 5_655 ?
O7 Cs2 O7 68.2(3) 7_565 3_645 ?
O16 Cs2 O7 46.5(2) 5_655 3_645 ?
O14 Cs2 O7 101.6(2) 8_755 3_645 ?
O6 Cs2 O7 104.0(3) . 3_645 ?
O19 Cs2 O7 148.9(4) 8_755 3_645 ?
O17 Cs2 O7 52.0(2) . 3_645 ?
O4 Cs2 O7 119.1(2) . 3_645 ?
O11 Cs2 O7 117.8(3) 1_545 3_645 ?
O17 Cs2 O7 40.4(2) 5_655 3_645 ?
O7 Cs2 O20 103.6(3) 7_565 . ?
O16 Cs2 O20 127.3(3) 5_655 . ?
O14 Cs2 O20 85.2(3) 8_755 . ?
O6 Cs2 O20 81.0(3) . . ?
O19 Cs2 O20 47.4(4) 8_755 . ?
O17 Cs2 O20 132.9(3) . . ?
O4 Cs2 O20 52.8(2) . . ?
O11 Cs2 O20 46.8(3) 1_545 . ?
O17 Cs2 O20 123.2(3) 5_655 . ?
O7 Cs2 O20 163.5(2) 3_645 . ?
O7 Cs2 Mo5 80.85(17) 7_565 5_655 ?
O16 Cs2 Mo5 23.2(3) 5_655 5_655 ?
O14 Cs2 Mo5 88.4(2) 8_755 5_655 ?
O6 Cs2 Mo5 129.9(2) . 5_655 ?
O19 Cs2 Mo5 161.3(3) 8_755 5_655 ?
O17 Cs2 Mo5 80.3(2) . 5_655 ?
O4 Cs2 Mo5 121.92(16) . 5_655 ?
O11 Cs2 Mo5 91.6(2) 1_545 5_655 ?
O17 Cs2 Mo5 28.85(17) 5_655 5_655 ?
O7 Cs2 Mo5 29.39(14) 3_645 5_655 ?
O20 Cs2 Mo5 138.01(19) . 5_655 ?
O15 Cs3 O15 79.8(4) 5_666 3_656 ?
O15 Cs3 O14 105.7(3) 5_666 8_766 ?
O15 Cs3 O14 87.9(3) 3_656 8_766 ?
O15 Cs3 O14 87.9(3) 5_666 2_665 ?
O15 Cs3 O14 105.7(3) 3_656 2_665 ?
O14 Cs3 O14 27.7(4) 8_766 2_665 ?
O15 Cs3 O9 77.2(3) 5_666 . ?
O15 Cs3 O9 113.7(3) 3_656 . ?
O14 Cs3 O9 158.2(3) 8_766 . ?
O14 Cs3 O9 134.1(3) 2_665 . ?
O15 Cs3 O9 113.7(3) 5_666 7_575 ?
O15 Cs3 O9 77.2(3) 3_656 7_575 ?
O14 Cs3 O9 134.1(3) 8_766 7_575 ?
O14 Cs3 O9 158.2(3) 2_665 7_575 ?
O9 Cs3 O9 58.2(4) . 7_575 ?
O15 Cs3 O19 162.9(4) 5_666 7_575 ?
O15 Cs3 O19 112.2(4) 3_656 7_575 ?
O14 Cs3 O19 87.3(4) 8_766 7_575 ?
O14 Cs3 O19 99.7(3) 2_665 7_575 ?
O9 Cs3 O19 86.7(4) . 7_575 ?
O9 Cs3 O19 60.2(3) 7_575 7_575 ?
O15 Cs3 O19 112.2(4) 5_666 . ?
O15 Cs3 O19 162.9(4) 3_656 . ?
O14 Cs3 O19 99.7(3) 8_766 . ?
O14 Cs3 O19 87.3(4) 2_665 . ?
O9 Cs3 O19 60.2(3) . . ?
O9 Cs3 O19 86.7(4) 7_575 . ?
O19 Cs3 O19 53.6(7) 7_575 . ?
O15 Cs3 O18 62.1(3) 5_666 . ?
O15 Cs3 O18 62.1(3) 3_656 . ?
O14 Cs3 O18 148.6(3) 8_766 . ?
O14 Cs3 O18 148.6(3) 2_665 . ?
O9 Cs3 O18 52.1(2) . . ?
O9 Cs3 O18 52.1(2) 7_575 . ?
O19 Cs3 O18 111.6(3) 7_575 . ?
O19 Cs3 O18 111.6(3) . . ?
O15 Cs3 O10 51.6(3) 5_666 . ?
O15 Cs3 O10 128.3(3) 3_656 . ?
O14 Cs3 O10 118.3(3) 8_766 . ?
O14 Cs3 O10 90.7(3) 2_665 . ?
O9 Cs3 O10 46.3(2) . . ?
O9 Cs3 O10 104.5(2) 7_575 . ?
O19 Cs3 O10 112.6(4) 7_575 . ?
O19 Cs3 O10 60.9(3) . . ?
O18 Cs3 O10 78.35(17) . . ?
O15 Cs3 O10 128.3(3) 5_666 7_575 ?
O15 Cs3 O10 51.6(3) 3_656 7_575 ?
O14 Cs3 O10 90.7(3) 8_766 7_575 ?
O14 Cs3 O10 118.3(3) 2_665 7_575 ?
O9 Cs3 O10 104.5(2) . 7_575 ?
O9 Cs3 O10 46.3(2) 7_575 7_575 ?
O19 Cs3 O10 60.9(3) 7_575 7_575 ?
O19 Cs3 O10 112.6(4) . 7_575 ?
O18 Cs3 O10 78.35(17) . 7_575 ?
O10 Cs3 O10 150.6(3) . 7_575 ?
O15 Cs3 O16 55.3(2) 5_666 5_666 ?
O15 Cs3 O16 55.3(2) 3_656 5_666 ?
O14 Cs3 O16 58.0(3) 8_766 5_666 ?
O14 Cs3 O16 58.0(3) 2_665 5_666 ?
O9 Cs3 O16 131.9(2) . 5_666 ?
O9 Cs3 O16 131.9(2) 7_575 5_666 ?
O19 Cs3 O16 141.3(4) 7_575 5_666 ?
O19 Cs3 O16 141.3(4) . 5_666 ?
O18 Cs3 O16 94.6(3) . 5_666 ?
O10 Cs3 O16 99.77(15) . 5_666 ?
O10 Cs3 O16 99.77(15) 7_575 5_666 ?
Mo4 O1 Mo2 98.8(3) . . ?
Mo4 O1 Mo2 98.8(3) . 7_565 ?
Mo2 O1 Mo2 150.1(6) . 7_565 ?
Mo4 O1 Mo1 99.6(5) . . ?
Mo2 O1 Mo1 100.3(3) . . ?
Mo2 O1 Mo1 100.3(3) 7_565 . ?
Mo5 O2 Mo3 96.5(3) . . ?
Mo5 O2 Mo3 96.5(3) . 7_565 ?
Mo3 O2 Mo3 155.4(6) . 7_565 ?
Mo5 O2 Mo1 99.4(5) . . ?
Mo3 O2 Mo1 99.1(3) . . ?
Mo3 O2 Mo1 99.1(3) 7_565 . ?
Mo2 O3 Mo4 109.3(4) . . ?
Mo1 O4 Mo3 112.3(4) . 7_565 ?
Mo1 O4 Mo2 111.9(4) . 7_565 ?
Mo3 O4 Mo2 91.7(3) 7_565 7_565 ?
Mo1 O4 Cs2 96.9(3) . . ?
Mo3 O4 Cs2 89.9(3) 7_565 . ?
Mo2 O4 Cs2 148.0(4) 7_565 . ?
Mo2 O5 Mo3 114.5(4) . . ?
Mo1 O6 Mo5 105.4(6) . . ?
Mo1 O6 Cs2 107.7(2) . 7_565 ?
Mo5 O6 Cs2 91.2(3) . 7_565 ?
Mo1 O6 Cs2 107.7(2) . . ?
Mo5 O6 Cs2 91.2(3) . . ?
Cs2 O6 Cs2 142.5(4) 7_565 . ?
Mo3 O7 Mo5 111.0(4) . . ?
Mo3 O7 Cs2 116.8(4) . 7_565 ?
Mo5 O7 Cs2 112.3(4) . 7_565 ?
Mo3 O7 Cs2 117.4(4) . 3_655 ?
Mo5 O7 Cs2 82.7(3) . 3_655 ?
Cs2 O7 Cs2 111.8(3) 7_565 3_655 ?
Mo1 O8 Mo4 106.1(6) . . ?
Mo1 O8 Cs3 161.2(6) . 2_664 ?
Mo4 O8 Cs3 92.7(4) . 2_664 ?
Mo2 O9 Mn1 141.7(5) . . ?
Mo2 O9 Cs3 112.4(4) . . ?
Mn1 O9 Cs3 96.8(3) . . ?
Mo2 O10 Cs1 133.3(5) . . ?
Mo2 O10 Cs3 96.6(4) . . ?
Cs1 O10 Cs3 118.1(3) . . ?
Mn1 O11 Cs2 112.1(5) . 7_565 ?
Mn1 O11 Cs2 112.1(5) . 1_565 ?
Cs2 O11 Cs2 80.8(3) 7_565 1_565 ?
Mo3 O12 Mn1 144.3(5) . . ?
Mo3 O12 Cs1 109.8(4) . 5_666 ?
Mn1 O12 Cs1 96.9(3) . 5_666 ?
O14 O14 Mo4 67.7(3) 7_565 . ?
O14 O14 Cs3 76.2(2) 7_565 2_664 ?
Mo4 O14 Cs3 124.0(4) . 2_664 ?
O14 O14 Cs2 120.4(2) 7_565 8_766 ?
Mo4 O14 Cs2 121.5(5) . 8_766 ?
Cs3 O14 Cs2 113.3(3) 2_664 8_766 ?
Mo3 O15 Cs3 145.2(6) . 5_666 ?
Mo3 O15 Cs1 94.1(4) . 5_666 ?
Cs3 O15 Cs1 120.6(3) 5_666 5_666 ?
Mo5 O16 Cs2 111.5(4) . 5_655 ?
Mo5 O16 Cs2 111.5(4) . 3_655 ?
Cs2 O16 Cs2 99.3(4) 5_655 3_655 ?
Mo5 O16 Cs3 128.7(6) . 5_666 ?
Cs2 O16 Cs3 100.9(3) 5_655 5_666 ?
Cs2 O16 Cs3 100.9(3) 3_655 5_666 ?
O17 O17 Mo5 68.1(4) 7_565 . ?
O17 O17 Cs1 77.0(2) 7_565 1_554 ?
Mo5 O17 Cs1 140.5(6) . 1_554 ?
O17 O17 Cs2 134.5(2) 7_565 . ?
Mo5 O17 Cs2 97.8(4) . . ?
Cs1 O17 Cs2 93.5(3) 1_554 . ?
O17 O17 Cs2 116.54(19) 7_565 5_655 ?
Mo5 O17 Cs2 87.1(4) . 5_655 ?
Cs1 O17 Cs2 126.0(3) 1_554 5_655 ?
Cs2 O17 Cs2 105.0(3) . 5_655 ?
Mn1 O18 Cs1 84.8(4) . 5_666 ?
Mn1 O18 Cs3 84.5(4) . . ?
Cs1 O18 Cs3 169.3(4) 5_666 . ?
Cs2 O19 Cs3 158.2(6) 8_766 . ?
O22 O22 Cs1 79.2(10) 7_565 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O8 1.723(13) . ?
Mo1 O6 1.734(13) . ?
Mo1 O4 1.858(9) . ?
Mo1 O4 1.858(9) 7_565 ?
Mo1 O1 2.305(11) . ?
Mo1 O2 2.314(12) . ?
Mo1 Cs2 4.1240(14) 7_565 ?
Mo1 Cs2 4.1240(14) . ?
Mo2 O10 1.684(9) . ?
Mo2 O9 1.760(10) . ?
Mo2 O5 1.908(9) . ?
Mo2 O3 1.941(9) . ?
Mo2 O1 2.171(3) . ?
Mo2 O4 2.281(8) 7_565 ?
Mo2 Mo4 3.2058(15) . ?
Mo2 Cs3 4.1925(13) . ?
Mo2 Cs1 4.3553(17) . ?
Mo3 O15 1.691(10) . ?
Mo3 O12 1.742(10) . ?
Mo3 O7 1.881(10) . ?
Mo3 O5 1.965(9) . ?
Mo3 O2 2.189(3) . ?
Mo3 O4 2.260(9) 7_565 ?
Mo3 Mo5 3.1726(14) . ?
Mo3 Cs1 4.0004(14) 5_666 ?
Mo3 Cs2 4.1326(17) 7_565 ?
Mo4 O13 1.676(13) . ?
Mo4 O14 1.957(10) 7_565 ?
Mo4 O14 1.957(10) . ?
Mo4 O3 1.989(10) . ?
Mo4 O3 1.989(10) 7_565 ?
Mo4 O1 2.049(12) . ?
Mo4 O8 2.410(12) . ?
Mo4 Cs2 4.4623(17) 8_766 ?
Mo4 Cs2 4.4622(17) 2_655 ?
Mo4 Cs3 4.503(2) 2_664 ?
Mo5 O16 1.684(14) . ?
Mo5 O17 1.923(11) 7_565 ?
Mo5 O17 1.923(11) . ?
Mo5 O7 1.968(9) . ?
Mo5 O7 1.969(9) 7_565 ?
Mo5 O2 2.061(12) . ?
Mo5 O6 2.433(13) . ?
Mo5 Cs2 3.9796(17) 5_655 ?
Mo5 Cs2 3.9796(17) 3_655 ?
Mo5 Cs2 4.1004(16) 7_565 ?
Mn1 O9 2.119(10) . ?
Mn1 O9 2.119(10) 7_575 ?
Mn1 O12 2.127(10) 7_575 ?
Mn1 O12 2.127(10) . ?
Mn1 O11 2.199(16) . ?
Mn1 O18 2.202(13) . ?
Mn1 Cs1 3.929(3) 5_666 ?
Mn1 Cs3 4.036(3) . ?
Cs1 O22 2.97(5) 7_565 ?
Cs1 O22 2.97(5) . ?
Cs1 O10 3.024(10) 7_565 ?
Cs1 O10 3.024(10) . ?
Cs1 O12 3.059(10) 3_646 ?
Cs1 O12 3.059(10) 5_666 ?
Cs1 O17 3.202(12) 7_566 ?
Cs1 O17 3.202(12) 1_556 ?
Cs1 O18 3.461(15) 5_666 ?
Cs1 O15 3.507(11) 3_646 ?
Cs1 O15 3.507(11) 5_666 ?
Cs2 O7 2.927(9) 7_565 ?
Cs2 O16 3.042(8) 5_655 ?
Cs2 O14 3.116(10) 8_755 ?
Cs2 O6 3.252(4) . ?
Cs2 O19 3.313(17) 8_755 ?
Cs2 O17 3.369(12) . ?
Cs2 O4 3.465(9) . ?
Cs2 O11 3.579(12) 1_545 ?
Cs2 O17 3.584(12) 5_655 ?
Cs2 O7 3.716(9) 3_645 ?
Cs2 O20 3.720(12) . ?
Cs3 O15 3.088(11) 5_666 ?
Cs3 O15 3.088(11) 3_656 ?
Cs3 O14 3.105(11) 8_766 ?
Cs3 O14 3.105(11) 2_665 ?
Cs3 O9 3.193(10) . ?
Cs3 O9 3.193(10) 7_575 ?
Cs3 O19 3.458(16) 7_575 ?
Cs3 O19 3.458(16) . ?
Cs3 O18 3.600(15) . ?
Cs3 O10 3.652(11) . ?
Cs3 O10 3.652(11) 7_575 ?
Cs3 O16 3.680(15) 5_666 ?
O14 O14 1.48(2) 7_565 ?
O17 O17 1.44(2) 7_565 ?
O22 O22 1.12(11) 7_565 ?
